#------------------------------------------------------------------------------
#$Date: 2016-09-10 02:17:19 +0300 (Sat, 10 Sep 2016) $
#$Revision: 186350 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/22/58/7225878.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7225878
loop_
_publ_author_name
'Najafi, Atefeh'
'Mirzaei, Masoud'
'Mague, Joel T.'
_publ_section_title
;
 Structural scope of six new layered to pillar-layered hybrid
 inorganic--organic networks bearing [BW12O40]5−and
 lanthanoid-cluster; database study toward ligand role in assemblies
;
_journal_issue                   35
_journal_name_full               CrystEngComm
_journal_page_first              6724
_journal_paper_doi               10.1039/C6CE01183G
_journal_volume                  18
_journal_year                    2016
_chemical_absolute_configuration unk
_chemical_formula_moiety         'C28 H44 N4 O32 Sm4, K, B O40 W12, 2(H2 O)'
_chemical_formula_sum            'C28 H48 B K N4 O74 Sm4 W12'
_chemical_formula_weight         4482.21
_space_group_crystal_system      monoclinic
_space_group_IT_number           9
_space_group_name_Hall           'C -2yc'
_space_group_name_H-M_alt        'C 1 c 1'
_symmetry_space_group_name_Hall  'C -2yc'
_symmetry_space_group_name_H-M   'C 1 c 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-03-11 deposited with the CCDC.
2016-07-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 132.839(1)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   30.270(3)
_cell_length_b                   15.5104(13)
_cell_length_c                   21.842(3)
_cell_measurement_reflns_used    9114
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      29.052
_cell_measurement_theta_min      2.482
_cell_volume                     7519.5(14)
_computing_cell_refinement       'SAINT (Bruker, 2015)'
_computing_data_collection       'APEX2 (Bruker, 2015)'
_computing_data_reduction        'SAINT (Bruker, 2015)'
_computing_molecular_graphics    'DIAMOND (Brandenburg & Putz, 2012)'
_computing_publication_material  'SHELXTL (Bruker, 2015)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2015a)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 8.3660
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'Bruker Smart APEX CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0556
_diffrn_reflns_av_unetI/netI     0.0574
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.982
_diffrn_reflns_limit_h_max       41
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            68697
_diffrn_reflns_point_group_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.982
_diffrn_reflns_theta_full        29.000
_diffrn_reflns_theta_max         29.121
_diffrn_reflns_theta_min         1.835
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    21.528
_exptl_absorpt_correction_T_max  0.31
_exptl_absorpt_correction_T_min  0.14
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'SADABS (Bruker, 2015)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.959
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             7984
_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent'
_exptl_crystal_size_max          0.155
_exptl_crystal_size_mid          0.139
_exptl_crystal_size_min          0.071
_exptl_transmission_factor_max   0.544
_exptl_transmission_factor_min   0.246
_refine_diff_density_max         17.554
_refine_diff_density_min         -9.049
_refine_diff_density_rms         0.570
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.48(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1112
_refine_ls_number_reflns         19433
_refine_ls_number_restraints     638
_refine_ls_restrained_S_all      1.074
_refine_ls_R_factor_all          0.0703
_refine_ls_R_factor_gt           0.0647
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0020P)²+1767.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1336
_refine_ls_wR_factor_ref         0.1375
_reflns_Friedel_coverage         0.999
_reflns_Friedel_fraction_full    0.990
_reflns_Friedel_fraction_max     0.982
_reflns_number_gt                18009
_reflns_number_total             19433
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c6ce01183g2.cif
_cod_data_source_block           jtm460_b
_cod_depositor_comments
'Adding full bibliography for 7225877--7225882.cif.'
_cod_database_code               7225878
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.135
_shelx_estimated_absorpt_t_max   0.310
_solvent_exptl_crystal_recrystallization_method water
loop_
_space_group_symop_operation_xyz
'x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Sm1 Sm 0.67424(7) 0.62822(10) 0.49620(9) 0.0062(3) Uani 1 1 d . .
Sm2 Sm 0.39583(7) 0.63852(10) 0.30970(10) 0.0082(3) Uani 1 1 d . .
Sm3 Sm 0.33593(7) 0.37311(10) 0.46842(9) 0.0062(3) Uani 1 1 d . .
Sm4 Sm 0.61644(7) 0.35994(10) 0.65588(10) 0.0076(3) Uani 1 1 d . .
O1 O 0.7534(11) 0.7276(16) 0.6100(15) 0.013(5) Uani 1 1 d . U
O2 O 0.7842(11) 0.8475(16) 0.6835(15) 0.014(5) Uani 1 1 d . U
O3 O 0.5652(11) 0.6447(15) 0.4054(15) 0.011(5) Uani 1 1 d . U
O4 O 0.4848(11) 0.7167(16) 0.3637(16) 0.015(5) Uani 1 1 d . U
O5 O 0.6436(10) 0.7432(14) 0.3864(13) 0.007(4) Uani 1 1 d . U
H5A H 0.6057 0.7370 0.3416 0.011 Uiso 1 1 d R U
H5B H 0.6653 0.7365 0.3740 0.011 Uiso 1 1 d R U
O6 O 0.7531(11) 0.6562(17) 0.4938(16) 0.015(5) Uani 1 1 d . U
H6A H 0.7571 0.7116 0.4925 0.023 Uiso 1 1 d R U
H6B H 0.7430 0.6325 0.4497 0.023 Uiso 1 1 d R U
O7 O 0.7534(12) 0.5253(18) 0.5871(18) 0.022(6) Uani 1 1 d . U
H7A H 0.7408 0.4857 0.6005 0.034 Uiso 1 1 d R U
H7B H 0.7844 0.5515 0.6321 0.034 Uiso 1 1 d R U
O8 O 0.6238(12) 0.4854(17) 0.4663(17) 0.017(5) Uani 1 1 d . U
H8A H 0.6101 0.4659 0.4187 0.026 Uiso 1 1 d R U
H8B H 0.5941 0.4917 0.4639 0.026 Uiso 1 1 d R U
O9 O 0.3931(10) 0.6162(15) 0.1962(14) 0.009(4) Uani 1 1 d . U
O10 O 0.3555(13) 0.5499(19) 0.0796(18) 0.024(6) Uani 1 1 d . U
O11 O 0.3716(11) 0.5343(15) 0.3670(15) 0.012(5) Uani 1 1 d . U
O12 O 0.3318(11) 0.4070(16) 0.3595(15) 0.013(5) Uani 1 1 d . U
O13 O 0.3486(12) 0.7131(18) 0.3489(17) 0.020(5) Uani 1 1 d . U
H13A H 0.3174 0.6838 0.3317 0.030 Uiso 1 1 d R U
H13B H 0.3371 0.7639 0.3259 0.030 Uiso 1 1 d R U
O14 O 0.3718(14) 0.780(2) 0.246(2) 0.029(6) Uani 1 1 d . U
H14A H 0.4041 0.8119 0.2763 0.043 Uiso 1 1 d R U
H14B H 0.3446 0.8044 0.2435 0.043 Uiso 1 1 d R U
O15 O 0.4791(11) 0.5198(15) 0.3663(15) 0.014(5) Uani 1 1 d . U
H15A H 0.4649 0.4692 0.3623 0.020 Uiso 1 1 d R U
H15B H 0.5109 0.5304 0.4183 0.020 Uiso 1 1 d R U
O16 O 0.4737(13) 0.6363(18) 0.4684(18) 0.023(6) Uani 1 1 d . U
H16A H 0.4860 0.5837 0.4861 0.034 Uiso 1 1 d R U
H16B H 0.4570 0.6559 0.4860 0.034 Uiso 1 1 d R U
O17 O 0.2580(10) 0.2754(14) 0.3567(14) 0.008(4) Uani 1 1 d . U
O18 O 0.2259(11) 0.1522(16) 0.2770(15) 0.012(4) Uani 1 1 d . U
O19 O 0.4471(12) 0.3539(17) 0.5629(17) 0.018(5) Uani 1 1 d . U
O20 O 0.5265(11) 0.2867(16) 0.6040(15) 0.013(5) Uani 1 1 d . U
O21 O 0.3707(11) 0.2623(16) 0.5864(16) 0.015(5) Uani 1 1 d . U
H21A H 0.3689 0.2101 0.5701 0.023 Uiso 1 1 d R U
H21B H 0.3471 0.2667 0.5957 0.023 Uiso 1 1 d R U
O22 O 0.2564(10) 0.3409(16) 0.4712(16) 0.013(5) Uani 1 1 d . U
H22A H 0.2530 0.2854 0.4723 0.019 Uiso 1 1 d R U
H22B H 0.2222 0.3621 0.4266 0.019 Uiso 1 1 d R U
O23 O 0.2534(13) 0.4767(18) 0.3773(18) 0.022(6) Uani 1 1 d . U
H23A H 0.2197 0.4531 0.3570 0.032 Uiso 1 1 d R U
H23B H 0.2510 0.4913 0.3367 0.032 Uiso 1 1 d R U
O24 O 0.3859(13) 0.5158(18) 0.4991(18) 0.022(6) Uani 1 1 d . U
H24A H 0.3996 0.5351 0.5467 0.033 Uiso 1 1 d R U
H24B H 0.3600 0.5523 0.4598 0.033 Uiso 1 1 d R U
O25 O 0.6183(11) 0.3823(16) 0.7676(15) 0.012(5) Uani 1 1 d . U
O26 O 0.6550(11) 0.4517(16) 0.8860(16) 0.014(5) Uani 1 1 d . U
O27 O 0.6400(11) 0.4688(16) 0.6008(16) 0.014(5) Uani 1 1 d . U
O28 O 0.6761(11) 0.5985(16) 0.6068(15) 0.014(5) Uani 1 1 d . U
O29 O 0.6690(13) 0.2847(19) 0.6195(19) 0.026(6) Uani 1 1 d . U
H29A H 0.7071 0.2802 0.6638 0.039 Uiso 1 1 d R U
H29B H 0.6644 0.3143 0.5816 0.039 Uiso 1 1 d R U
O30 O 0.6389(12) 0.2176(18) 0.7211(18) 0.022(6) Uani 1 1 d . U
H30A H 0.6059 0.1874 0.6918 0.033 Uiso 1 1 d R U
H30B H 0.6534 0.2243 0.7714 0.033 Uiso 1 1 d R U
O31 O 0.5330(12) 0.4797(17) 0.5980(17) 0.020(6) Uani 1 1 d . U
H31A H 0.5470 0.5299 0.6008 0.030 Uiso 1 1 d R U
H31B H 0.5238 0.4800 0.6280 0.030 Uiso 1 1 d R U
O32 O 0.5390(15) 0.362(2) 0.498(2) 0.029(7) Uani 1 1 d . U
H32A H 0.5279 0.3093 0.4791 0.043 Uiso 1 1 d R U
H32B H 0.5543 0.3852 0.4794 0.043 Uiso 1 1 d R U
N1 N 0.6387(12) 0.7656(18) 0.5170(17) 0.008(5) Uani 1 1 d . U
N2 N 0.3459(11) 0.5031(17) 0.2283(15) 0.005(4) Uani 1 1 d . U
N3 N 0.3697(11) 0.2368(17) 0.4459(16) 0.007(5) Uani 1 1 d . U
N4 N 0.6657(11) 0.4971(18) 0.7397(16) 0.006(5) Uani 1 1 d . U
C1 C 0.7441(12) 0.7946(18) 0.6276(17) 0.003(5) Uani 1 1 d . U
C2 C 0.6788(14) 0.824(2) 0.5747(19) 0.007(5) Uani 1 1 d . U
C3 C 0.6596(15) 0.897(2) 0.586(2) 0.010(6) Uani 1 1 d . U
H3 H 0.6886 0.9359 0.6292 0.012 Uiso 1 1 calc R U
C4 C 0.5992(16) 0.914(2) 0.537(2) 0.015(7) Uani 1 1 d . U
H4 H 0.5860 0.9655 0.5443 0.017 Uiso 1 1 calc R U
C5 C 0.5593(13) 0.8545(19) 0.4785(19) 0.005(5) Uani 1 1 d . U
H5 H 0.5172 0.8624 0.4441 0.007 Uiso 1 1 calc R U
C6 C 0.5816(15) 0.782(2) 0.470(2) 0.013(6) Uani 1 1 d . U
C7 C 0.5407(14) 0.709(2) 0.408(2) 0.010(6) Uani 1 1 d . U
C8 C 0.3632(14) 0.560(2) 0.1431(19) 0.007(5) Uani 1 1 d . U
C9 C 0.3343(13) 0.4866(19) 0.1571(18) 0.005(5) Uani 1 1 d . U
C10 C 0.2960(14) 0.429(2) 0.103(2) 0.010(6) Uani 1 1 d . U
H10 H 0.2871 0.4257 0.0524 0.012 Uiso 1 1 calc R U
C11 C 0.2700(14) 0.378(2) 0.114(2) 0.010(6) Uani 1 1 d . U
H11 H 0.2438 0.3352 0.0739 0.011 Uiso 1 1 calc R U
C12 C 0.2808(16) 0.387(2) 0.191(2) 0.015(7) Uani 1 1 d . U
H12 H 0.2610 0.3510 0.2017 0.018 Uiso 1 1 calc R U
C13 C 0.3216(15) 0.449(2) 0.247(2) 0.011(6) Uani 1 1 d . U
C14 C 0.3437(16) 0.464(2) 0.331(2) 0.017(7) Uani 1 1 d . U
C15 C 0.2651(12) 0.1995(18) 0.3350(17) 0.003(5) Uani 1 1 d . U
C16 C 0.3327(13) 0.181(2) 0.3870(19) 0.006(5) Uani 1 1 d . U
C17 C 0.3510(14) 0.104(2) 0.3767(19) 0.007(5) Uani 1 1 d . U
H17 H 0.3224 0.0637 0.3352 0.009 Uiso 1 1 calc R U
C18 C 0.4112(15) 0.090(2) 0.428(2) 0.013(6) Uani 1 1 d . U
H18 H 0.4251 0.0385 0.4226 0.015 Uiso 1 1 calc R U
C19 C 0.4527(17) 0.150(2) 0.489(2) 0.018(7) Uani 1 1 d . U
H19 H 0.4947 0.1402 0.5240 0.021 Uiso 1 1 calc R U
C20 C 0.4313(12) 0.2248(18) 0.4970(17) 0.003(5) Uani 1 1 d . U
C21 C 0.4719(13) 0.2924(19) 0.5573(19) 0.006(5) Uani 1 1 d . U
C22 C 0.6470(14) 0.4452(19) 0.8209(19) 0.006(5) Uani 1 1 d . U
C23 C 0.6781(16) 0.507(2) 0.810(2) 0.017(7) Uani 1 1 d . U
C24 C 0.7188(14) 0.572(2) 0.8710(19) 0.007(5) Uani 1 1 d . U
H24 H 0.7272 0.5802 0.9212 0.009 Uiso 1 1 calc R U
C25 C 0.7461(15) 0.625(2) 0.848(2) 0.012(6) Uani 1 1 d . U
H25 H 0.7739 0.6697 0.8843 0.014 Uiso 1 1 calc R U
C26 C 0.7317(18) 0.611(3) 0.777(2) 0.019(7) Uani 1 1 d . U
H26 H 0.7509 0.6438 0.7635 0.023 Uiso 1 1 calc R U
C27 C 0.6891(13) 0.550(2) 0.7208(19) 0.006(5) Uani 1 1 d . U
C28 C 0.6675(13) 0.541(2) 0.6370(19) 0.006(5) Uani 1 1 d . U
K1 K 0.5078(4) 0.3649(4) 0.7335(6) 0.0147(11) Uani 1 1 d . .
W1 W 0.49126(6) -0.35901(8) 0.72485(9) 0.0192(3) Uani 1 1 d . .
W2 W 0.37066(6) -0.24437(9) 0.57701(9) 0.0187(3) Uani 1 1 d . .
W3 W 0.42492(6) -0.24796(10) 0.77158(8) 0.0150(3) Uani 1 1 d . .
W4 W 0.57983(7) -0.24755(9) 0.68969(8) 0.0151(3) Uani 1 1 d . .
W5 W 0.45408(6) -0.13674(8) 0.53450(7) 0.0078(2) Uani 1 1 d . .
W6 W 0.37936(6) -0.01188(11) 0.57946(8) 0.0172(3) Uani 1 1 d . .
W7 W 0.42764(6) -0.01598(11) 0.77118(8) 0.0166(3) Uani 1 1 d . .
W8 W 0.56082(6) -0.13436(8) 0.93639(8) 0.0083(2) Uani 1 1 d . .
W9 W 0.63300(6) -0.25038(9) 0.89569(8) 0.0180(3) Uani 1 1 d . .
W10 W 0.58154(6) -0.03011(10) 0.69012(8) 0.0157(3) Uani 1 1 d . .
W11 W 0.50528(7) 0.08991(7) 0.73590(10) 0.0124(2) Uani 1 1 d . .
W12 W 0.63770(6) -0.03554(10) 0.89862(8) 0.0174(3) Uani 1 1 d . .
O33 O 0.5244(9) 0.1955(14) 0.7468(14) 0.012(4) Uani 1 1 d . U
O34 O 0.3168(11) 0.0382(17) 0.4945(16) 0.018(5) Uani 1 1 d . U
O35 O 0.3906(11) 0.0305(16) 0.7946(16) 0.017(5) Uani 1 1 d . U
O36 O 0.3883(12) -0.2850(18) 0.8004(17) 0.023(5) Uani 1 1 d . U
O37 O 0.3014(11) -0.2813(16) 0.4844(16) 0.020(5) Uani 1 1 d . U
O38 O 0.4166(11) -0.1378(16) 0.4316(16) 0.019(5) Uani 1 1 d . U
O39 O 0.6229(12) 0.0326(18) 0.6823(17) 0.021(6) Uani 1 1 d . U
O40 O 0.6995(10) 0.0307(15) 0.9691(14) 0.011(4) Uani 1 1 d . U
O41 O 0.5766(13) -0.1377(17) 1.0274(17) 0.023(6) Uani 1 1 d . U
O42 O 0.5003(12) -0.4673(13) 0.7304(18) 0.015(4) Uani 1 1 d . U
O43 O 0.6122(14) -0.317(2) 0.6743(19) 0.032(6) Uani 1 1 d . U
O44 O 0.6895(11) -0.3222(16) 0.9651(15) 0.018(5) Uani 1 1 d . U
O45 O 0.4287(10) 0.0956(15) 0.6287(14) 0.013(4) Uani 1 1 d . U
O46 O 0.4660(11) 0.0883(16) 0.7772(15) 0.019(5) Uani 1 1 d . U
O47 O 0.5760(11) 0.0473(16) 0.8407(16) 0.020(5) Uani 1 1 d . U
O48 O 0.5358(11) 0.0502(17) 0.6888(16) 0.020(5) Uani 1 1 d . U
O49 O 0.3655(11) 0.0119(17) 0.6531(16) 0.021(5) Uani 1 1 d . U
O50 O 0.4005(11) -0.1293(16) 0.7531(15) 0.017(5) Uani 1 1 d . U
O51 O 0.5003(11) -0.0493(16) 0.8767(15) 0.017(5) Uani 1 1 d . U
O52 O 0.5163(11) -0.0546(17) 0.5735(16) 0.019(5) Uani 1 1 d . U
O53 O 0.6320(10) -0.0382(15) 0.8083(14) 0.014(4) Uani 1 1 d . U
O54 O 0.6158(11) -0.1432(16) 0.6979(15) 0.018(5) Uani 1 1 d . U
O55 O 0.6215(10) -0.0560(15) 0.9692(15) 0.015(4) Uani 1 1 d . U
O56 O 0.6775(10) -0.1473(14) 0.9343(14) 0.011(4) Uani 1 1 d . U
O57 O 0.6156(10) -0.2258(15) 0.9645(14) 0.014(4) Uani 1 1 d . U
O58 O 0.4990(10) -0.2197(15) 0.8755(14) 0.013(4) Uani 1 1 d . U
O59 O 0.3580(12) -0.2593(17) 0.6516(16) 0.023(5) Uani 1 1 d . U
O60 O 0.4545(12) -0.3565(17) 0.7704(16) 0.023(5) Uani 1 1 d . U
O61 O 0.4116(12) -0.3513(17) 0.6150(17) 0.025(5) Uani 1 1 d . U
O62 O 0.5241(12) -0.3233(18) 0.6813(17) 0.025(6) Uani 1 1 d . U
O63 O 0.6280(11) -0.2496(16) 0.8058(15) 0.017(5) Uani 1 1 d . U
O64 O 0.5114(10) -0.2246(15) 0.5700(15) 0.015(5) Uani 1 1 d . U
O65 O 0.4176(10) -0.0468(15) 0.5435(14) 0.015(4) Uani 1 1 d . U
O66 O 0.4076(10) -0.2163(15) 0.5376(15) 0.015(5) Uani 1 1 d . U
O67 O 0.5650(11) -0.3258(17) 0.8331(16) 0.021(5) Uani 1 1 d . U
O68 O 0.3509(11) -0.1243(16) 0.5665(16) 0.019(5) Uani 1 1 d . U
B1 B 0.5115(16) -0.134(2) 0.736(3) 0.013 Uani 1 1 d . .
O69 O 0.4698(9) -0.0523(12) 0.7151(12) 0.005(4) Uani 1 1 d . U
O70 O 0.4622(10) -0.2130(14) 0.7090(14) 0.012(4) Uani 1 1 d . U
O71 O 0.5221(9) -0.1387(14) 0.6841(13) 0.010(4) Uani 1 1 d . U
O72 O 0.5595(10) -0.1387(15) 0.8269(14) 0.016(4) Uani 1 1 d . U
O73 O 0.7490(12) 0.1476(18) 0.3294(18) 0.020(5) Uani 1 1 d . U
H73A H 0.7504 0.0948 0.3442 0.030 Uiso 1 1 d R U
H73B H 0.7640 0.1822 0.3710 0.030 Uiso 1 1 d R U
O74 O 0.7618(14) 0.358(2) 0.637(2) 0.030(7) Uani 1 1 d . U
H74A H 0.7507 0.3533 0.5887 0.044 Uiso 1 1 d R U
H74B H 0.7992 0.3420 0.6746 0.044 Uiso 1 1 d R U
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O7 Sm1 O26 84.9(9) . 2_564
O7 Sm1 O28 73.4(9) . .
O26 Sm1 O28 136.6(9) 2_564 .
O7 Sm1 O3 141.0(9) . .
O26 Sm1 O3 88.1(8) 2_564 .
O28 Sm1 O3 86.1(8) . .
O7 Sm1 O6 72.4(9) . .
O26 Sm1 O6 69.4(9) 2_564 .
O28 Sm1 O6 133.6(8) . .
O3 Sm1 O6 139.2(8) . .
O7 Sm1 O1 81.0(9) . .
O26 Sm1 O1 137.2(8) 2_564 .
O28 Sm1 O1 76.6(8) . .
O3 Sm1 O1 126.6(8) . .
O6 Sm1 O1 67.9(8) . .
O7 Sm1 O8 73.5(9) . .
O26 Sm1 O8 66.0(9) 2_564 .
O28 Sm1 O8 71.9(9) . .
O3 Sm1 O8 68.6(8) . .
O6 Sm1 O8 125.2(9) . .
O1 Sm1 O8 143.9(8) . .
O7 Sm1 N1 135.1(9) . .
O26 Sm1 N1 139.7(9) 2_564 .
O28 Sm1 N1 73.1(8) . .
O3 Sm1 N1 63.9(8) . .
O6 Sm1 N1 112.8(9) . .
O1 Sm1 N1 62.8(8) . .
O8 Sm1 N1 121.7(9) . .
O7 Sm1 O5 138.5(8) . .
O26 Sm1 O5 74.8(8) 2_564 .
O28 Sm1 O5 143.3(8) . .
O3 Sm1 O5 75.0(8) . .
O6 Sm1 O5 66.6(8) . .
O1 Sm1 O5 89.6(8) . .
O8 Sm1 O5 126.3(8) . .
N1 Sm1 O5 70.4(8) . .
O7 Sm1 K1 135.7(7) . 2_564
O26 Sm1 K1 54.4(6) 2_564 2_564
O28 Sm1 K1 122.7(6) . 2_564
O3 Sm1 K1 38.4(6) . 2_564
O6 Sm1 K1 103.7(6) . 2_564
O1 Sm1 K1 139.9(6) . 2_564
O8 Sm1 K1 74.0(6) . 2_564
N1 Sm1 K1 88.0(6) . 2_564
O5 Sm1 K1 53.2(5) . 2_564
O13 Sm2 O4 108.7(9) . .
O13 Sm2 O14 75.5(11) . .
O4 Sm2 O14 68.0(9) . .
O13 Sm2 O11 71.1(9) . .
O4 Sm2 O11 135.1(8) . .
O14 Sm2 O11 144.4(10) . .
O13 Sm2 O9 144.1(9) . .
O4 Sm2 O9 79.8(8) . .
O14 Sm2 O9 76.0(10) . .
O11 Sm2 O9 127.6(8) . .
O13 Sm2 N2 116.2(9) . .
O4 Sm2 N2 135.1(8) . .
O14 Sm2 N2 123.6(10) . .
O11 Sm2 N2 63.9(8) . .
O9 Sm2 N2 64.6(8) . .
O13 Sm2 O2 70.7(8) . 4_464
O4 Sm2 O2 135.4(8) . 4_464
O14 Sm2 O2 69.0(9) . 4_464
O11 Sm2 O2 88.3(8) . 4_464
O9 Sm2 O2 79.0(8) . 4_464
N2 Sm2 O2 65.3(8) . 4_464
O13 Sm2 O16 75.3(9) . .
O4 Sm2 O16 69.4(9) . .
O14 Sm2 O16 115.6(10) . .
O11 Sm2 O16 67.4(9) . .
O9 Sm2 O16 137.8(9) . .
N2 Sm2 O16 120.8(9) . .
O2 Sm2 O16 143.1(9) 4_464 .
O13 Sm2 O15 140.8(8) . .
O4 Sm2 O15 74.3(8) . .
O14 Sm2 O15 135.5(9) . .
O11 Sm2 O15 79.8(8) . .
O9 Sm2 O15 75.0(8) . .
N2 Sm2 O15 70.7(8) . .
O2 Sm2 O15 135.2(8) 4_464 .
O16 Sm2 O15 69.4(9) . .
O12 Sm3 O10 136.1(9) . 2_565
O12 Sm3 O17 77.2(8) . .
O10 Sm3 O17 136.6(9) 2_565 .
O12 Sm3 O23 73.1(9) . .
O10 Sm3 O23 84.8(10) 2_565 .
O17 Sm3 O23 80.6(8) . .
O12 Sm3 O19 88.7(9) . .
O10 Sm3 O19 87.5(9) 2_565 .
O17 Sm3 O19 126.5(8) . .
O23 Sm3 O19 143.7(9) . .
O12 Sm3 O22 132.7(8) . .
O10 Sm3 O22 69.7(9) 2_565 .
O17 Sm3 O22 66.9(8) . .
O23 Sm3 O22 71.6(9) . .
O19 Sm3 O22 137.4(8) . .
O12 Sm3 O24 71.4(9) . .
O10 Sm3 O24 66.3(10) 2_565 .
O17 Sm3 O24 144.4(8) . .
O23 Sm3 O24 74.6(9) . .
O19 Sm3 O24 69.8(9) . .
O22 Sm3 O24 125.9(9) . .
O12 Sm3 N3 75.0(8) . .
O10 Sm3 N3 139.4(9) 2_565 .
O17 Sm3 N3 62.2(8) . .
O23 Sm3 N3 135.3(9) . .
O19 Sm3 N3 64.3(9) . .
O22 Sm3 N3 111.1(8) . .
O24 Sm3 N3 122.6(9) . .
O12 Sm3 O21 147.2(8) . .
O10 Sm3 O21 71.1(9) 2_565 .
O17 Sm3 O21 92.5(8) . .
O23 Sm3 O21 136.6(9) . .
O19 Sm3 O21 72.4(8) . .
O22 Sm3 O21 66.4(8) . .
O24 Sm3 O21 123.1(8) . .
N3 Sm3 O21 72.7(8) . .
O20 Sm4 O25 77.7(8) . .
O20 Sm4 O27 135.2(8) . .
O25 Sm4 O27 125.5(8) . .
O20 Sm4 O30 68.1(9) . .
O25 Sm4 O30 74.8(9) . .
O27 Sm4 O30 147.9(9) . .
O20 Sm4 O18 137.1(8) . 4
O25 Sm4 O18 80.6(8) . 4
O27 Sm4 O18 87.3(8) . 4
O30 Sm4 O18 70.7(8) . 4
O20 Sm4 O29 113.0(9) . .
O25 Sm4 O29 143.3(9) . .
O27 Sm4 O29 72.8(9) . .
O30 Sm4 O29 77.2(10) . .
O18 Sm4 O29 68.0(9) 4 .
O20 Sm4 N4 131.3(8) . .
O25 Sm4 N4 63.4(8) . .
O27 Sm4 N4 63.2(8) . .
O30 Sm4 N4 122.8(9) . .
O18 Sm4 N4 65.6(8) 4 .
O29 Sm4 N4 115.7(9) . .
O20 Sm4 O32 70.2(9) . .
O25 Sm4 O32 137.5(9) . .
O27 Sm4 O32 68.3(9) . .
O30 Sm4 O32 115.8(10) . .
O18 Sm4 O32 141.8(9) 4 .
O29 Sm4 O32 76.7(10) . .
N4 Sm4 O32 121.4(9) . .
O20 Sm4 O31 72.6(8) . .
O25 Sm4 O31 75.2(8) . .
O27 Sm4 O31 77.5(8) . .
O30 Sm4 O31 134.5(9) . .
O18 Sm4 O31 135.3(8) 4 .
O29 Sm4 O31 141.1(9) . .
N4 Sm4 O31 70.1(8) . .
O32 Sm4 O31 69.2(10) . .
C1 O1 Sm1 125(2) . .
C1 O2 Sm2 143(2) . 4_565
C7 O3 Sm1 124(2) . .
C7 O3 K1 104(2) . 2_564
Sm1 O3 K1 109.8(9) . 2_564
C7 O4 Sm2 143(2) . .
Sm1 O5 H5A 109.4 . .
Sm1 O5 H5B 109.5 . .
H5A O5 H5B 109.5 . .
Sm1 O6 H6A 109.4 . .
Sm1 O6 H6B 109.4 . .
H6A O6 H6B 109.5 . .
Sm1 O7 H7A 109.2 . .
Sm1 O7 H7B 109.1 . .
H7A O7 H7B 109.5 . .
Sm1 O8 H8A 109.2 . .
Sm1 O8 H8B 109.7 . .
H8A O8 H8B 109.5 . .
C8 O9 Sm2 124(2) . .
C8 O9 K1 107.5(19) . 2_564
Sm2 O9 K1 118.5(9) . 2_564
C8 O10 Sm3 143(2) . 2_564
C14 O11 Sm2 124(2) . .
C14 O12 Sm3 144(2) . .
Sm2 O13 H13A 109.2 . .
Sm2 O13 H13B 109.3 . .
H13A O13 H13B 109.5 . .
Sm2 O14 H14A 109.3 . .
Sm2 O14 H14B 109.1 . .
H14A O14 H14B 109.5 . .
Sm2 O15 H15A 109.2 . .
Sm2 O15 H15B 109.4 . .
H15A O15 H15B 109.5 . .
Sm2 O16 H16A 109.7 . .
Sm2 O16 H16B 108.5 . .
H16A O16 H16B 109.5 . .
C15 O17 Sm3 128.2(18) . .
C15 O18 Sm4 144(2) . 4_454
C21 O19 Sm3 124(2) . .
C21 O19 K1 106(2) . .
Sm3 O19 K1 112.7(10) . .
C21 O20 Sm4 145(2) . .
Sm3 O21 H21A 109.5 . .
Sm3 O21 H21B 109.3 . .
H21A O21 H21B 109.5 . .
Sm3 O22 H22A 109.3 . .
Sm3 O22 H22B 109.3 . .
H22A O22 H22B 109.5 . .
Sm3 O23 H23A 109.5 . .
Sm3 O23 H23B 109.3 . .
H23A O23 H23B 109.5 . .
Sm3 O24 H24A 109.5 . .
Sm3 O24 H24B 109.7 . .
H24A O24 H24B 109.5 . .
C22 O25 Sm4 123.6(19) . .
C22 O25 K1 104.5(18) . .
Sm4 O25 K1 119.6(9) . .
C22 O26 Sm1 144(2) . 2_565
C28 O27 Sm4 125(2) . .
C28 O28 Sm1 143(2) . .
Sm4 O29 H29A 109.5 . .
Sm4 O29 H29B 109.3 . .
H29A O29 H29B 109.5 . .
Sm4 O30 H30A 109.3 . .
Sm4 O30 H30B 109.1 . .
H30A O30 H30B 109.5 . .
Sm4 O31 H31A 109.3 . .
Sm4 O31 H31B 109.4 . .
H31A O31 H31B 109.5 . .
Sm4 O32 H32A 109.3 . .
Sm4 O32 H32B 110.1 . .
H32A O32 H32B 109.5 . .
C6 N1 C2 118(3) . .
C6 N1 Sm1 121(2) . .
C2 N1 Sm1 121(2) . .
C13 N2 C9 117(3) . .
C13 N2 Sm2 120(2) . .
C9 N2 Sm2 122.2(19) . .
C16 N3 C20 119(3) . .
C16 N3 Sm3 124(2) . .
C20 N3 Sm3 117.0(19) . .
C23 N4 C27 120(3) . .
C23 N4 Sm4 120(2) . .
C27 N4 Sm4 118(2) . .
O1 C1 O2 126(3) . .
O1 C1 C2 119(3) . .
O2 C1 C2 115(3) . .
N1 C2 C3 120(3) . .
N1 C2 C1 112(3) . .
C3 C2 C1 127(3) . .
C2 C3 C4 122(3) . .
C2 C3 H3 119.1 . .
C4 C3 H3 119.1 . .
C5 C4 C3 117(3) . .
C5 C4 H4 121.4 . .
C3 C4 H4 121.4 . .
C4 C5 C6 118(3) . .
C4 C5 H5 120.8 . .
C6 C5 H5 120.8 . .
N1 C6 C5 124(3) . .
N1 C6 C7 113(3) . .
C5 C6 C7 123(3) . .
O4 C7 O3 124(3) . .
O4 C7 C6 118(3) . .
O3 C7 C6 118(3) . .
O4 C7 K1 87(2) . 2_564
O3 C7 K1 54.6(17) . 2_564
C6 C7 K1 133(2) . 2_564
O9 C8 O10 127(3) . .
O9 C8 C9 119(3) . .
O10 C8 C9 115(3) . .
C10 C9 N2 123(3) . .
C10 C9 C8 126(3) . .
N2 C9 C8 110(2) . .
C11 C10 C9 124(3) . .
C11 C10 H10 118.1 . .
C9 C10 H10 118.1 . .
C10 C11 C12 119(3) . .
C10 C11 H11 120.6 . .
C12 C11 H11 120.6 . .
C13 C12 C11 116(3) . .
C13 C12 H12 122.2 . .
C11 C12 H12 122.2 . .
N2 C13 C12 121(3) . .
N2 C13 C14 114(3) . .
C12 C13 C14 125(3) . .
O12 C14 O11 126(3) . .
O12 C14 C13 117(3) . .
O11 C14 C13 116(3) . .
O18 C15 O17 128(3) . .
O18 C15 C16 121(3) . .
O17 C15 C16 111(2) . .
N3 C16 C17 124(3) . .
N3 C16 C15 115(3) . .
C17 C16 C15 121(3) . .
C18 C17 C16 118(3) . .
C18 C17 H17 121.2 . .
C16 C17 H17 121.2 . .
C17 C18 C19 121(3) . .
C17 C18 H18 119.6 . .
C19 C18 H18 119.6 . .
C18 C19 C20 119(3) . .
C18 C19 H19 120.7 . .
C20 C19 H19 120.7 . .
N3 C20 C19 120(3) . .
N3 C20 C21 118(3) . .
C19 C20 C21 122(3) . .
O20 C21 O19 122(3) . .
O20 C21 C20 122(3) . .
O19 C21 C20 116(3) . .
O26 C22 O25 124(3) . .
O26 C22 C23 118(3) . .
O25 C22 C23 117(3) . .
N4 C23 C24 123(3) . .
N4 C23 C22 114(3) . .
C24 C23 C22 123(3) . .
C23 C24 C25 114(3) . .
C23 C24 H24 123.2 . .
C25 C24 H24 123.2 . .
C26 C25 C24 120(3) . .
C26 C25 H25 120.1 . .
C24 C25 H25 120.1 . .
C25 C26 C27 121(3) . .
C25 C26 H26 119.4 . .
C27 C26 H26 119.4 . .
N4 C27 C26 122(3) . .
N4 C27 C28 117(3) . .
C26 C27 C28 122(3) . .
O28 C28 O27 125(3) . .
O28 C28 C27 121(3) . .
O27 C28 C27 114(3) . .
O42 K1 O33 175.6(9) 1_565 .
O42 K1 O19 93.4(9) 1_565 .
O33 K1 O19 89.4(8) . .
O42 K1 O3 92.9(9) 1_565 2_565
O33 K1 O3 84.5(7) . 2_565
O19 K1 O3 173.2(6) . 2_565
O42 K1 O25 88.8(8) 1_565 .
O33 K1 O25 88.0(7) . .
O19 K1 O25 87.0(8) . .
O3 K1 O25 95.8(7) 2_565 .
O42 K1 O9 80.3(8) 1_565 2_565
O33 K1 O9 103.0(7) . 2_565
O19 K1 O9 93.0(8) . 2_565
O3 K1 O9 85.4(7) 2_565 2_565
O25 K1 O9 169.0(5) . 2_565
O42 K1 C7 108.6(9) 1_565 2_565
O33 K1 C7 69.7(8) . 2_565
O19 K1 C7 152.3(8) . 2_565
O3 K1 C7 21.2(7) 2_565 2_565
O25 K1 C7 109.5(8) . 2_565
O9 K1 C7 75.0(7) 2_565 2_565
O42 K1 Sm1 90.7(7) 1_565 2_565
O33 K1 Sm1 85.2(5) . 2_565
O19 K1 Sm1 150.6(6) . 2_565
O3 K1 Sm1 31.9(5) 2_565 2_565
O25 K1 Sm1 64.0(5) . 2_565
O9 K1 Sm1 116.4(5) 2_565 2_565
C7 K1 Sm1 48.8(6) 2_565 2_565
O42 W1 O62 102.4(13) . .
O42 W1 O67 100.5(12) . .
O62 W1 O67 88.4(11) . .
O42 W1 O61 98.9(12) . .
O62 W1 O61 89.8(12) . .
O67 W1 O61 160.4(11) . .
O42 W1 O60 96.0(12) . .
O62 W1 O60 161.6(12) . .
O67 W1 O60 87.4(11) . .
O61 W1 O60 88.2(11) . .
O42 W1 O70 170.1(10) . .
O62 W1 O70 85.2(10) . .
O67 W1 O70 85.9(9) . .
O61 W1 O70 74.5(10) . .
O60 W1 O70 76.6(10) . .
O37 W2 O66 99.5(11) . .
O37 W2 O61 97.7(12) . .
O66 W2 O61 89.3(11) . .
O37 W2 O68 98.5(11) . .
O66 W2 O68 87.4(10) . .
O61 W2 O68 163.8(11) . .
O37 W2 O59 99.7(11) . .
O66 W2 O59 160.8(11) . .
O61 W2 O59 88.3(11) . .
O68 W2 O59 89.6(11) . .
O37 W2 O70 171.5(10) . .
O66 W2 O70 86.6(9) . .
O61 W2 O70 76.4(10) . .
O68 W2 O70 87.5(9) . .
O59 W2 O70 74.3(10) . .
O36 W3 O58 100.2(11) . .
O36 W3 O60 97.8(12) . .
O58 W3 O60 92.2(11) . .
O36 W3 O50 98.4(12) . .
O58 W3 O50 90.2(10) . .
O60 W3 O50 162.9(11) . .
O36 W3 O59 97.1(12) . .
O58 W3 O59 162.5(11) . .
O60 W3 O59 88.3(11) . .
O50 W3 O59 84.5(11) . .
O36 W3 O70 169.1(11) . .
O58 W3 O70 89.9(9) . .
O60 W3 O70 77.4(9) . .
O50 W3 O70 85.7(9) . .
O59 W3 O70 73.1(9) . .
O43 W4 O63 104.0(13) . .
O43 W4 O54 101.5(13) . .
O63 W4 O54 91.0(11) . .
O43 W4 O62 100.5(14) . .
O63 W4 O62 86.8(11) . .
O54 W4 O62 157.8(11) . .
O43 W4 O64 94.8(12) . .
O63 W4 O64 160.7(10) . .
O54 W4 O64 89.4(10) . .
O62 W4 O64 85.5(11) . .
O43 W4 O71 168.6(12) . .
O63 W4 O71 87.1(9) . .
O54 W4 O71 75.6(9) . .
O62 W4 O71 82.2(9) . .
O64 W4 O71 74.3(9) . .
O38 W5 O65 103.7(11) . .
O38 W5 O66 101.3(11) . .
O65 W5 O66 88.6(10) . .
O38 W5 O64 97.8(11) . .
O65 W5 O64 158.2(10) . .
O66 W5 O64 90.7(10) . .
O38 W5 O52 99.5(11) . .
O65 W5 O52 86.0(10) . .
O66 W5 O52 159.2(10) . .
O64 W5 O52 87.0(10) . .
O38 W5 O71 170.4(10) . .
O65 W5 O71 83.5(9) . .
O66 W5 O71 85.1(9) . .
O64 W5 O71 74.7(9) . .
O52 W5 O71 74.4(9) . .
O34 W6 O65 102.9(11) . .
O34 W6 O68 101.8(12) . .
O65 W6 O68 91.1(10) . .
O34 W6 O49 96.3(12) . .
O65 W6 O49 160.5(10) . .
O68 W6 O49 88.1(11) . .
O34 W6 O45 94.4(11) . .
O65 W6 O45 91.1(9) . .
O68 W6 O45 162.7(10) . .
O49 W6 O45 84.2(10) . .
O34 W6 O69 166.5(10) . .
O65 W6 O69 85.9(8) . .
O68 W6 O69 88.0(9) . .
O49 W6 O69 74.5(9) . .
O45 W6 O69 75.1(8) . .
O35 W7 O50 100.4(12) . .
O35 W7 O51 102.2(11) . .
O50 W7 O51 88.9(11) . .
O35 W7 O46 96.5(12) . .
O50 W7 O46 162.9(10) . .
O51 W7 O46 89.9(11) . .
O35 W7 O49 93.7(11) . .
O50 W7 O49 92.2(11) . .
O51 W7 O49 163.5(11) . .
O46 W7 O49 84.2(11) . .
O35 W7 O69 165.8(10) . .
O50 W7 O69 88.9(9) . .
O51 W7 O69 88.6(9) . .
O46 W7 O69 74.0(9) . .
O49 W7 O69 75.0(9) . .
O41 W8 O51 101.4(12) . .
O41 W8 O55 98.5(12) . .
O51 W8 O55 92.8(10) . .
O41 W8 O58 99.0(12) . .
O51 W8 O58 88.4(10) . .
O55 W8 O58 161.9(10) . .
O41 W8 O57 96.2(12) . .
O51 W8 O57 162.2(10) . .
O55 W8 O57 87.1(10) . .
O58 W8 O57 86.3(10) . .
O41 W8 O72 168.3(11) . .
O51 W8 O72 88.9(9) . .
O55 W8 O72 75.3(9) . .
O58 W8 O72 86.6(9) . .
O57 W8 O72 73.9(9) . .
O44 W9 O63 104.7(11) . .
O44 W9 O56 100.2(11) . .
O63 W9 O56 89.3(10) . .
O44 W9 O67 100.1(11) . .
O63 W9 O67 88.5(11) . .
O56 W9 O67 159.5(10) . .
O44 W9 O57 94.3(10) . .
O63 W9 O57 161.0(10) . .
O56 W9 O57 88.6(9) . .
O67 W9 O57 86.9(10) . .
O44 W9 O72 166.8(10) . .
O63 W9 O72 87.7(9) . .
O56 W9 O72 75.0(9) . .
O67 W9 O72 84.5(10) . .
O57 W9 O72 73.5(9) . .
O39 W10 O48 102.1(12) . .
O39 W10 O53 102.1(12) . .
O48 W10 O53 88.2(10) . .
O39 W10 O52 98.3(12) . .
O48 W10 O52 91.7(11) . .
O53 W10 O52 159.2(10) . .
O39 W10 O54 98.0(12) . .
O48 W10 O54 159.9(11) . .
O53 W10 O54 86.2(10) . .
O52 W10 O54 86.9(11) . .
O39 W10 O71 168.7(11) . .
O48 W10 O71 87.0(9) . .
O53 W10 O71 84.7(9) . .
O52 W10 O71 74.5(9) . .
O54 W10 O71 73.3(9) . .
O33 W11 O45 98.3(10) . .
O33 W11 O48 98.3(11) . .
O45 W11 O48 89.0(10) . .
O33 W11 O47 99.7(11) . .
O45 W11 O47 161.9(11) . .
O48 W11 O47 88.6(11) . .
O33 W11 O46 102.0(11) . .
O45 W11 O46 87.2(10) . .
O48 W11 O46 159.7(12) . .
O47 W11 O46 88.8(10) . .
O33 W11 O69 174.7(8) . .
O45 W11 O69 77.8(9) . .
O48 W11 O69 85.3(9) . .
O47 W11 O69 84.2(9) . .
O46 W11 O69 74.5(9) . .
O40 W12 O53 102.8(11) . .
O40 W12 O47 99.8(11) . .
O53 W12 O47 88.2(10) . .
O40 W12 O55 95.4(11) . .
O53 W12 O55 161.8(10) . .
O47 W12 O55 88.5(10) . .
O40 W12 O56 99.9(10) . .
O53 W12 O56 89.4(10) . .
O47 W12 O56 160.2(10) . .
O55 W12 O56 87.6(9) . .
O40 W12 O72 168.5(10) . .
O53 W12 O72 87.3(9) . .
O47 W12 O72 85.8(10) . .
O55 W12 O72 74.6(9) . .
O56 W12 O72 74.4(9) . .
W11 O33 K1 156.6(11) . .
W1 O42 K1 176.8(15) . 1_545
W11 O45 W6 118.2(12) . .
W11 O46 W7 120.8(13) . .
W12 O47 W11 147.2(15) . .
W10 O48 W11 148.0(15) . .
W7 O49 W6 119.7(13) . .
W7 O50 W3 143.8(14) . .
W7 O51 W8 145.0(14) . .
W10 O52 W5 122.0(13) . .
W12 O53 W10 147.6(13) . .
W4 O54 W10 121.1(13) . .
W8 O55 W12 120.6(12) . .
W9 O56 W12 121.2(11) . .
W8 O57 W9 121.5(12) . .
W3 O58 W8 144.4(13) . .
W2 O59 W3 120.3(14) . .
W3 O60 W1 117.5(13) . .
W2 O61 W1 119.5(14) . .
W1 O62 W4 148.5(16) . .
W9 O63 W4 148.7(14) . .
W5 O64 W4 120.9(12) . .
W6 O65 W5 147.2(13) . .
W2 O66 W5 148.7(14) . .
W9 O67 W1 146.4(14) . .
W6 O68 W2 143.9(14) . .
O71 B1 O72 123(3) . .
O71 B1 O69 112(3) . .
O72 B1 O69 107(3) . .
O71 B1 O70 108(3) . .
O72 B1 O70 106(3) . .
O69 B1 O70 98(2) . .
B1 O69 W11 120.9(16) . .
B1 O69 W7 129.0(19) . .
W11 O69 W7 90.7(7) . .
B1 O69 W6 125.3(18) . .
W11 O69 W6 88.9(6) . .
W7 O69 W6 90.7(7) . .
B1 O70 W2 127.7(18) . .
B1 O70 W3 128.2(19) . .
W2 O70 W3 92.0(8) . .
B1 O70 W1 119.2(16) . .
W2 O70 W1 89.5(8) . .
W3 O70 W1 88.4(8) . .
B1 O71 W4 124.8(19) . .
B1 O71 W10 120.3(19) . .
W4 O71 W10 89.9(7) . .
B1 O71 W5 131(2) . .
W4 O71 W5 90.0(7) . .
W10 O71 W5 89.0(7) . .
B1 O72 W12 119.5(19) . .
B1 O72 W8 133(2) . .
W12 O72 W8 89.4(8) . .
B1 O72 W9 122.3(19) . .
W12 O72 W9 89.4(8) . .
W8 O72 W9 90.9(8) . .
H73A O73 H73B 109.5 . .
H74A O74 H74B 107.1 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sm1 O7 2.40(3) .
Sm1 O26 2.40(3) 2_564
Sm1 O28 2.42(2) .
Sm1 O3 2.45(2) .
Sm1 O6 2.46(3) .
Sm1 O1 2.49(2) .
Sm1 O8 2.51(3) .
Sm1 N1 2.56(3) .
Sm1 O5 2.60(2) .
Sm1 K1 4.360(10) 2_564
Sm2 O13 2.40(3) .
Sm2 O4 2.41(2) .
Sm2 O14 2.43(3) .
Sm2 O11 2.44(2) .
Sm2 O9 2.45(2) .
Sm2 N2 2.49(3) .
Sm2 O2 2.53(2) 4_464
Sm2 O16 2.54(3) .
Sm2 O15 2.65(2) .
Sm3 O12 2.35(2) .
Sm3 O10 2.39(3) 2_565
Sm3 O17 2.45(2) .
Sm3 O23 2.45(3) .
Sm3 O19 2.50(3) .
Sm3 O22 2.50(2) .
Sm3 O24 2.50(3) .
Sm3 N3 2.54(3) .
Sm3 O21 2.65(2) .
Sm4 O20 2.41(2) .
Sm4 O25 2.43(2) .
Sm4 O27 2.44(3) .
Sm4 O30 2.46(3) .
Sm4 O18 2.47(2) 4
Sm4 O29 2.50(3) .
Sm4 N4 2.53(3) .
Sm4 O32 2.53(3) .
Sm4 O31 2.66(3) .
O1 C1 1.21(4) .
O2 C1 1.27(4) .
O2 Sm2 2.53(2) 4_565
O3 C7 1.27(4) .
O3 K1 2.87(3) 2_564
O4 C7 1.26(4) .
O5 H5A 0.8700 .
O5 H5B 0.8698 .
O6 H6A 0.8701 .
O6 H6B 0.8700 .
O7 H7A 0.8701 .
O7 H7B 0.8700 .
O8 H8A 0.8699 .
O8 H8B 0.8701 .
O9 C8 1.23(4) .
O9 K1 2.99(2) 2_564
O10 C8 1.25(4) .
O10 Sm3 2.39(3) 2_564
O11 C14 1.27(4) .
O12 C14 1.26(4) .
O13 H13A 0.8701 .
O13 H13B 0.8701 .
O14 H14A 0.8698 .
O14 H14B 0.8702 .
O15 H15A 0.8699 .
O15 H15B 0.8700 .
O16 H16A 0.8700 .
O16 H16B 0.8701 .
O17 C15 1.34(3) .
O18 C15 1.23(4) .
O18 Sm4 2.47(2) 4_454
O19 C21 1.27(4) .
O19 K1 2.82(3) .
O20 C21 1.22(4) .
O21 H21A 0.8700 .
O21 H21B 0.8700 .
O22 H22A 0.8700 .
O22 H22B 0.8700 .
O23 H23A 0.8699 .
O23 H23B 0.8700 .
O24 H24A 0.8699 .
O24 H24B 0.8700 .
O25 C22 1.30(4) .
O25 K1 2.90(3) .
O26 C22 1.27(4) .
O26 Sm1 2.40(3) 2_565
O27 C28 1.29(4) .
O28 C28 1.24(4) .
O29 H29A 0.8699 .
O29 H29B 0.8700 .
O30 H30A 0.8700 .
O30 H30B 0.8699 .
O31 H31A 0.8701 .
O31 H31B 0.8699 .
O32 H32A 0.8700 .
O32 H32B 0.8698 .
N1 C6 1.30(4) .
N1 C2 1.35(4) .
N2 C13 1.34(4) .
N2 C9 1.37(4) .
N3 C16 1.31(4) .
N3 C20 1.39(4) .
N4 C23 1.31(4) .
N4 C27 1.32(4) .
C1 C2 1.53(4) .
C2 C3 1.36(4) .
C3 C4 1.38(5) .
C3 H3 0.9500 .
C4 C5 1.36(5) .
C4 H4 0.9500 .
C5 C6 1.39(4) .
C5 H5 0.9500 .
C6 C7 1.53(5) .
C7 K1 3.42(3) 2_564
C8 C9 1.58(4) .
C9 C10 1.29(4) .
C10 C11 1.25(4) .
C10 H10 0.9500 .
C11 C12 1.49(5) .
C11 H11 0.9500 .
C12 C13 1.38(5) .
C12 H12 0.9500 .
C13 C14 1.49(5) .
C15 C16 1.55(4) .
C16 C17 1.39(4) .
C17 C18 1.36(4) .
C17 H17 0.9500 .
C18 C19 1.39(5) .
C18 H18 0.9500 .
C19 C20 1.40(5) .
C19 H19 0.9500 .
C20 C21 1.46(4) .
C22 C23 1.47(5) .
C23 C24 1.45(5) .
C24 C25 1.48(4) .
C24 H24 0.9500 .
C25 C26 1.32(5) .
C25 H25 0.9500 .
C26 C27 1.38(5) .
C26 H26 0.9500 .
C27 C28 1.47(4) .
K1 O42 2.61(2) 1_565
K1 O33 2.65(2) .
K1 O3 2.87(3) 2_565
K1 O9 2.99(2) 2_565
K1 C7 3.42(3) 2_565
K1 Sm1 4.360(10) 2_565
W1 O42 1.69(2) .
W1 O62 1.87(3) .
W1 O67 1.91(3) .
W1 O61 1.93(3) .
W1 O60 1.93(3) .
W1 O70 2.37(2) .
W2 O37 1.75(2) .
W2 O66 1.87(2) .
W2 O61 1.89(3) .
W2 O68 1.92(2) .
W2 O59 1.92(3) .
W2 O70 2.32(2) .
W3 O36 1.70(2) .
W3 O58 1.86(2) .
W3 O60 1.92(3) .
W3 O50 1.92(2) .
W3 O59 1.94(3) .
W3 O70 2.35(2) .
W4 O43 1.64(3) .
W4 O63 1.88(2) .
W4 O54 1.89(2) .
W4 O62 1.96(3) .
W4 O64 1.97(2) .
W4 O71 2.37(2) .
W5 O38 1.69(3) .
W5 O65 1.87(2) .
W5 O66 1.91(2) .
W5 O64 1.91(2) .
W5 O52 1.93(2) .
W5 O71 2.40(2) .
W6 O34 1.69(3) .
W6 O65 1.87(2) .
W6 O68 1.88(2) .
W6 O49 1.95(2) .
W6 O45 2.00(2) .
W6 O69 2.375(19) .
W7 O35 1.68(3) .
W7 O50 1.87(2) .
W7 O51 1.88(2) .
W7 O46 1.94(3) .
W7 O49 1.94(3) .
W7 O69 2.361(19) .
W8 O41 1.70(3) .
W8 O51 1.88(2) .
W8 O55 1.89(2) .
W8 O58 1.91(2) .
W8 O57 1.94(2) .
W8 O72 2.37(2) .
W9 O44 1.71(2) .
W9 O63 1.86(2) .
W9 O56 1.88(2) .
W9 O67 1.91(3) .
W9 O57 1.94(2) .
W9 O72 2.38(2) .
W10 O39 1.68(3) .
W10 O48 1.85(3) .
W10 O53 1.91(2) .
W10 O52 1.92(3) .
W10 O54 1.98(3) .
W10 O71 2.40(2) .
W11 O33 1.70(2) .
W11 O45 1.87(2) .
W11 O48 1.89(2) .
W11 O47 1.90(3) .
W11 O46 1.92(2) .
W11 O69 2.359(19) .
W12 O40 1.73(2) .
W12 O53 1.86(2) .
W12 O47 1.88(2) .
W12 O55 1.94(2) .
W12 O56 1.95(2) .
W12 O72 2.36(2) .
O42 K1 2.61(2) 1_545
B1 O71 1.38(5) .
B1 O72 1.46(5) .
B1 O69 1.62(4) .
B1 O70 1.69(4) .
O73 H73A 0.8700 .
O73 H73B 0.8700 .
O74 H74A 0.8703 .
O74 H74B 0.8701 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O5 H5A O33 0.87 2.12 2.87(3) 144 2_564
O6 H6A O22 0.87 2.06 2.92(3) 172 3
O7 H7A O74 0.87 2.06 2.75(4) 136 .
O8 H8A O67 0.87 2.57 3.27(4) 138 2_554
O8 H8B O15 0.87 2.60 3.35(4) 145 .
O13 H13A O73 0.87 2.11 2.93(4) 155 3_455
O14 H14A O46 0.87 2.42 3.18(4) 146 2_564
O15 H15A O60 0.87 2.52 3.04(4) 119 2_554
O16 H16A O31 0.87 2.42 3.20(4) 148 .
O21 H21A O45 0.87 2.22 2.90(3) 135 .
O22 H22A O6 0.87 2.06 2.92(3) 171 3_445
O23 H23A O53 0.87 2.47 3.03(4) 123 4_454
O24 H24A O61 0.87 2.17 2.93(4) 145 1_565
O32 H32A O58 0.87 2.26 3.01(4) 144 2_554
C19 H19 O41 0.95 2.43 3.24(5) 144 2_554
C24 H24 O44 0.95 2.45 3.19(4) 135 1_565
O73 H73A O23 0.87 1.95 2.82(4) 180 3_545
O73 H73B O37 0.87 1.98 2.81(4) 158 3
O74 H74A O44 0.87 2.04 2.84(4) 152 2_554
O74 H74B O50 0.87 2.32 3.10(4) 149 3
